LMucko/crystallography-open-database huggingface dataset:
Cordierite I: The coordination of Fe2+ Sample: C005
Geiger, C. A.; Armbruster, T.; Khomenko, V.; Quartieri, S.; American Mineralogist 85 (2000) 1255–1264; doi:

data_9002410
_publ_section_title
;
 Cordierite I: The coordination of Fe2+
 Sample: C005
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1255
_journal_page_last               1264
_journal_volume                  85
_journal_year                    2000
_chemical_formula_sum            'C4 Al4 Mg2 O18 Si5'
_chemical_name_mineral           Cordierite
_space_group_IT_number           66
_symmetry_space_group_name_Hall  '-C 2 2c'
_symmetry_space_group_name_H-M   'C c c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   17.101
_cell_length_b                   9.736
_cell_length_c                   9.331
_cell_volume                     1553.568
_database_code_amcsd             0002495
_exptl_crystal_density_diffrn    2.706
_cod_original_formula_sum        'Si5 Al4 Mg2 C4 O18'
_cod_database_code               9002410
Crystal chemical variations in Li- and Fe-rich micas from Pikes Peak batholith (central Colorado) Sample: 114
Brigatti, M. F.; Lugli, C.; Poppi, L.; Foord, E. E.; Kile, D. E.; American Mineralogist 85 (2000) 1275–1286; doi:

data_9002411
_publ_section_title
;
 Crystal chemical variations in Li- and Fe-rich micas from
 Pikes Peak batholith (central Colorado)
 Sample: 114
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1275
_journal_page_last               1286
_journal_volume                  85
_journal_year                    2000
_chemical_formula_sum
;Al1.504 F1.746 Fe0.455 H0.142 K0.906 Li1.423 Mn0.038 Na0.005 O10.254 Rb0.051
 Si3.536
;
_chemical_name_mineral           Polylithionite
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.72
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.262
_cell_length_b                   9.085
_cell_length_c                   10.099
_cell_volume                     474.360
_database_code_amcsd             0002496
_exptl_crystal_density_diffrn    2.902
_cod_original_formula_sum
;Si3.536 Al1.504 Li1.423 Fe.455 Mn.038 Na.005 Rb.051 K.906 O10.254 F1.746
 H.142
;
_cod_database_code               9002411
Crystal chemical variations in Li- and Fe-rich micas from Pikes Peak batholith (central Colorado) Sample: 55a
Brigatti, M. F.; Lugli, C.; Poppi, L.; Foord, E. E.; Kile, D. E.; American Mineralogist 85 (2000) 1275–1286; doi:

data_9002412
_publ_section_title
;
 Crystal chemical variations in Li- and Fe-rich micas from
 Pikes Peak batholith (central Colorado)
 Sample: 55a
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1275
_journal_page_last               1286
_journal_volume                  85
_journal_year                    2000
_chemical_formula_sum
;Al1.7 F1.626 Fe0.589 H0.206 K0.94 Li1.129 Mg0.007 Mn0.038 Na0.002 O10.374
 Rb0.006 Si3.412
;
_chemical_name_mineral           Polylithionite
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.70
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.270
_cell_length_b                   9.092
_cell_length_c                   10.080
_cell_volume                     474.584
_database_code_amcsd             0002497
_exptl_crystal_density_diffrn    2.933
_cod_original_formula_sum
;Si3.412 Al1.7 Li1.129 Fe.589 Mg.007 Mn.038 Na.002 Rb.006 K.94 O10.374 F1.626
 H.206
;
_cod_database_code               9002412
Crystal chemical variations in Li- and Fe-rich micas from Pikes Peak batholith (central Colorado) Sample: 55b
Brigatti, M. F.; Lugli, C.; Poppi, L.; Foord, E. E.; Kile, D. E.; American Mineralogist 85 (2000) 1275–1286; doi:

data_9002413
_publ_section_title
;
 Crystal chemical variations in Li- and Fe-rich micas from
 Pikes Peak batholith (central Colorado)
 Sample: 55b
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1275
_journal_page_last               1286
_journal_volume                  85
_journal_year                    2000
_chemical_formula_sum
;Al1.649 F1.534 Fe0.608 H0.24 K0.956 Li1.222 Mg0.005 Mn0.045 Na0.011 O10.466
 Rb0.023 Si3.412
;
_chemical_name_mineral           Polylithionite
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.75
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.263
_cell_length_b                   9.085
_cell_length_c                   10.078
_cell_volume                     473.416
_database_code_amcsd             0002498
_exptl_crystal_density_diffrn    2.959
_cod_original_formula_sum
;Si3.412 Al1.649 Li1.222 Fe.608 Mg.005 Mn.045 Na.011 Rb.023 K.956 O10.466
 F1.534 H.24
;
_cod_database_code               9002413
Crystal chemical variations in Li- and Fe-rich micas from Pikes Peak batholith (central Colorado) sample: 130(1)
Brigatti, M. F.; Lugli, C.; Poppi, L.; Foord, E. E.; Kile, D. E.; American Mineralogist 85 (2000) 1275–1286; doi:

data_9002414
_publ_section_title
;
 Crystal chemical variations in Li- and Fe-rich micas from
 Pikes Peak batholith (central Colorado)
 sample: 130(1)
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1275
_journal_page_last               1286
_journal_volume                  85
_journal_year                    2000
_chemical_formula_sum
;Al1.705 Ca0.006 F1.552 Fe0.795 H0.186 K0.968 Li1.08 Mg0.022 Mn0.062 Na0.016
 O10.448 Si3.296
;
_chemical_name_mineral           Polylithionite
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.80
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.290
_cell_length_b                   9.128
_cell_length_c                   10.093
_cell_volume                     478.729
_database_code_amcsd             0002499
_exptl_crystal_density_diffrn    2.981
_cod_original_formula_sum
;Si3.296 Al1.705 Li1.08 Fe.795 Mg.022 Mn.062 Ca.006 Na.016 K.968 O10.448
 F1.552 H.186
;
_cod_database_code               9002414
Crystal chemical variations in Li- and Fe-rich micas from Pikes Peak batholith (central Colorado) sample: 130(2)
Brigatti, M. F.; Lugli, C.; Poppi, L.; Foord, E. E.; Kile, D. E.; American Mineralogist 85 (2000) 1275–1286; doi:

data_9002415
_publ_section_title
;
 Crystal chemical variations in Li- and Fe-rich micas from
 Pikes Peak batholith (central Colorado)
 sample: 130(2)
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1275
_journal_page_last               1286
_journal_volume                  85
_journal_year                    2000
_chemical_formula_sum
;Al1.69 Ca0.006 F1.544 Fe0.484 H0.186 K0.964 Li1.093 Mg0.022 Mn0.062 Na0.016
 O10.456 Si3.328
;
_chemical_name_mineral           Polylithionite
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.70
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.275
_cell_length_b                   9.105
_cell_length_c                   10.084
_cell_volume                     475.902
_database_code_amcsd             0002500
_exptl_crystal_density_diffrn    2.880
_cod_original_formula_sum
;Si3.328 Al1.69 Li1.093 Fe.484 Mg.022 Mn.062 Ca.006 Na.016 K.964 O10.456
 F1.544 H.186
;
_cod_database_code               9002415
Crystal chemical variations in Li- and Fe-rich micas from Pikes Peak batholith (central Colorado) Sample: 137
Brigatti, M. F.; Lugli, C.; Poppi, L.; Foord, E. E.; Kile, D. E.; American Mineralogist 85 (2000) 1275–1286; doi:

data_9002416
_publ_section_title
;
 Crystal chemical variations in Li- and Fe-rich micas from
 Pikes Peak batholith (central Colorado)
 Sample: 137
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1275
_journal_page_last               1286
_journal_volume                  85
_journal_year                    2000
_chemical_formula_sum
;Al1.84 F1.738 Fe0.748 H0.244 K0.944 Li0.973 Mg0.011 Mn0.073 Na0.023 O10.262
 Si3.208
;
_chemical_name_mineral           Polylithionite
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.79
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.279
_cell_length_b                   9.114
_cell_length_c                   10.077
_cell_volume                     476.261
_database_code_amcsd             0002501
_exptl_crystal_density_diffrn    2.981
_cod_original_formula_sum
'Si3.208 Al1.84 Li.973 Fe.748 Mg.011 Mn.073 Na.023 K.944 O10.262 F1.738 H.244'
_cod_database_code               9002416
Crystal chemical variations in Li- and Fe-rich micas from Pikes Peak batholith (central Colorado) Sample: 104
Brigatti, M. F.; Lugli, C.; Poppi, L.; Foord, E. E.; Kile, D. E.; American Mineralogist 85 (2000) 1275–1286; doi:

data_9002417
_publ_section_title
;
 Crystal chemical variations in Li- and Fe-rich micas from
 Pikes Peak batholith (central Colorado)
 Sample: 104
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1275
_journal_page_last               1286
_journal_volume                  85
_journal_year                    2000
_chemical_formula_sum
;Al1.732 Ca0.001 F1.606 Fe0.788 H0.244 K0.96 Li0.963 Mg0.009 Mn0.01 Na0.02
 O10.394 Si3.304
;
_chemical_name_mineral           Polylithionite
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.85
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.285
_cell_length_b                   9.122
_cell_length_c                   10.101
_cell_volume                     478.262
_database_code_amcsd             0002502
_exptl_crystal_density_diffrn    2.959
_cod_original_formula_sum
;Si3.304 Al1.732 Li.963 Fe.788 Mg.009 Mn.01 Ca.001 Na.02 K.96 O10.394 F1.606
 H.244
;
_cod_database_code               9002417
Crystal chemical variations in Li- and Fe-rich micas from Pikes Peak batholith (central Colorado) Sample: 54b
Brigatti, M. F.; Lugli, C.; Poppi, L.; Foord, E. E.; Kile, D. E.; American Mineralogist 85 (2000) 1275–1286; doi:

data_9002418
_publ_section_title
;
 Crystal chemical variations in Li- and Fe-rich micas from
 Pikes Peak batholith (central Colorado)
 Sample: 54b
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1275
_journal_page_last               1286
_journal_volume                  85
_journal_year                    2000
_chemical_formula_sum
;Al1.72 F1.654 Fe0.731 H0.244 K0.94 Li0.591 Mg0.008 Mn0.063 Na0.02 O10.346
 Rb0.004 Si3.308
;
_chemical_name_mineral           Polylithionite
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.76
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.283
_cell_length_b                   9.123
_cell_length_c                   10.072
_cell_volume                     476.903
_database_code_amcsd             0002503
_exptl_crystal_density_diffrn    2.943
_cod_original_formula_sum
;Si3.308 Al1.72 Li.591 Fe.731 Mg.008 Mn.063 Na.02 Rb.004 K.94 O10.346 F1.654
 H.244
;
_cod_database_code               9002418
Crystal chemical variations in Li- and Fe-rich micas from Pikes Peak batholith (central Colorado) Sample: 177
Brigatti, M. F.; Lugli, C.; Poppi, L.; Foord, E. E.; Kile, D. E.; American Mineralogist 85 (2000) 1275–1286; doi:

data_9002419
_publ_section_title
;
 Crystal chemical variations in Li- and Fe-rich micas from
 Pikes Peak batholith (central Colorado)
 Sample: 177
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1275
_journal_page_last               1286
_journal_volume                  85
_journal_year                    2000
_chemical_formula_sum
;Al1.645 F1.92 Fe0.887 H0.08 K0.942 Li0.862 Mg0.009 Mn0.064 Na0.04 O10.08
 Rb0.003 Si3.228 Ti0.01
;
_chemical_name_mineral           Polylithionite
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.81
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.288
_cell_length_b                   9.133
_cell_length_c                   10.088
_cell_volume                     478.557
_database_code_amcsd             0002504
_exptl_crystal_density_diffrn    2.988
_cod_original_formula_sum
;Si3.228 Al1.645 Li.862 Fe.887 Ti.01 Mg.009 Mn.064 Na.04 Rb.003 K.942 O10.08
 (F1.92 H.08)
;
_cod_database_code               9002419
Crystal chemical variations in Li- and Fe-rich micas from Pikes Peak batholith (central Colorado) sample: 140(1)
Brigatti, M. F.; Lugli, C.; Poppi, L.; Foord, E. E.; Kile, D. E.; American Mineralogist 85 (2000) 1275–1286; doi:

data_9002420
_publ_section_title
;
 Crystal chemical variations in Li- and Fe-rich micas from
 Pikes Peak batholith (central Colorado)
 sample: 140(1)
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1275
_journal_page_last               1286
_journal_volume                  85
_journal_year                    2000
_chemical_formula_sum
;Al1.838 F1.622 Fe0.868 H0.248 K0.958 Li0.853 Mg0.051 Mn0.058 Na0.014 O10.378
 Si3.176
;
_chemical_name_mineral           Polylithionite
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.78
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.283
_cell_length_b                   9.118
_cell_length_c                   10.092
_cell_volume                     477.557
_database_code_amcsd             0002505
_exptl_crystal_density_diffrn    3.008
_cod_original_formula_sum
'Si3.176 Al1.838 Li.853 Fe.868 Mg.051 Mn.058 Na.014 K.958 O10.378 F1.622 H.248'
_cod_database_code               9002420
Crystal chemical variations in Li- and Fe-rich micas from Pikes Peak batholith (central Colorado) sample: 140(2)
Brigatti, M. F.; Lugli, C.; Poppi, L.; Foord, E. E.; Kile, D. E.; American Mineralogist 85 (2000) 1275–1286; doi:

data_9002421
_publ_section_title
;
 Crystal chemical variations in Li- and Fe-rich micas from
 Pikes Peak batholith (central Colorado)
 sample: 140(2)
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1275
_journal_page_last               1286
_journal_volume                  85
_journal_year                    2000
_chemical_formula_sum
;Al1.743 F1.64 Fe0.879 H0.248 K0.954 Li0.849 Mg0.047 Mn0.06 Na0.014 O10.36
 Si3.236
;
_chemical_name_mineral           Siderophyllite
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.81
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.297
_cell_length_b                   9.146
_cell_length_c                   10.102
_cell_volume                     480.720
_database_code_amcsd             0002506
_exptl_crystal_density_diffrn    2.985
_cod_original_formula_sum
'Si3.236 Al1.743 Li.849 Fe.879 Mg.047 Mn.06 Na.014 K.954 O10.36 F1.64 H.248'
_cod_database_code               9002421
Crystal chemical variations in Li- and Fe-rich micas from Pikes Peak batholith (central Colorado) Sample: 24
Brigatti, M. F.; Lugli, C.; Poppi, L.; Foord, E. E.; Kile, D. E.; American Mineralogist 85 (2000) 1275–1286; doi:

data_9002422
_publ_section_title
;
 Crystal chemical variations in Li- and Fe-rich micas from
 Pikes Peak batholith (central Colorado)
 Sample: 24
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1275
_journal_page_last               1286
_journal_volume                  85
_journal_year                    2000
_chemical_formula_sum
;Al1.795 F1.59 Fe0.828 H0.174 K0.82 Li0.764 Mn0.078 Na0.034 O10.41 Rb0.092
 Si3.312
;
_chemical_name_mineral           Siderophyllite
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.83
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.295
_cell_length_b                   9.139
_cell_length_c                   10.077
_cell_volume                     478.951
_database_code_amcsd             0002507
_exptl_crystal_density_diffrn    3.016
_cod_original_formula_sum
'Si3.312 Al1.795 Li.764 Fe.828 Mn.078 Na.034 Rb.092 K.82 O10.41 F1.59 H.174'
_cod_database_code               9002422
Crystal chemical variations in Li- and Fe-rich micas from Pikes Peak batholith (central Colorado) Sample: 47
Brigatti, M. F.; Lugli, C.; Poppi, L.; Foord, E. E.; Kile, D. E.; American Mineralogist 85 (2000) 1275–1286; doi:

data_9002423
_publ_section_title
;
 Crystal chemical variations in Li- and Fe-rich micas from
 Pikes Peak batholith (central Colorado)
 Sample: 47
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1275
_journal_page_last               1286
_journal_volume                  85
_journal_year                    2000
_chemical_formula_sum
;Al1.753 F1.08 Fe1.48 H0.284 K0.986 Li0.416 Mg0.054 Mn0.078 Na0.014 O10.92
 Si3.056 Ti0.108
;
_chemical_name_mineral           Siderophyllite
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.73
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.339
_cell_length_b                   9.233
_cell_length_c                   10.135
_cell_volume                     490.869
_database_code_amcsd             0002508
_exptl_crystal_density_diffrn    3.138
_cod_original_formula_sum
;Si3.056 Al1.753 Li.416 Fe1.48 Mn.078 Ti.108 Mg.054 (Na.014 K.986) O10.92
 F1.08 H.284
;
_cod_database_code               9002423
Crystal chemical variations in Li- and Fe-rich micas from Pikes Peak batholith (central Colorado) Sample: 103
Brigatti, M. F.; Lugli, C.; Poppi, L.; Foord, E. E.; Kile, D. E.; American Mineralogist 85 (2000) 1275–1286; doi:

data_9002424
_publ_section_title
;
 Crystal chemical variations in Li- and Fe-rich micas from
 Pikes Peak batholith (central Colorado)
 Sample: 103
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1275
_journal_page_last               1286
_journal_volume                  85
_journal_year                    2000
_chemical_formula_sum
;Al1.678 F1.294 Fe1.314 H0.154 K0.985 Li0.621 Mg0.022 Mn0.051 Na0.036 O10.706
 Rb0.002 Si3.224
;
_chemical_name_mineral           Siderophyllite
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.74
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.300
_cell_length_b                   9.144
_cell_length_c                   10.089
_cell_volume                     480.380
_database_code_amcsd             0002509
_exptl_crystal_density_diffrn    3.128
_cod_original_formula_sum
;Si3.224 Al1.678 Li.621 Fe1.314 Mn.051 Mg.022 Na.036 Rb.002 K.985 O10.706
 F1.294 H.154
;
_cod_database_code               9002424
The crystal structure of TlAlSiO4: The role of inert pairs in exclusion of Tl from silicate minerals
Kyono, A.; Kimata, M.; Shimizu, M.; American Mineralogist 85 (2000) 1287–1293; doi:

data_9002425
_publ_section_title
;
 The crystal structure of TlAlSiO4: The role of inert pairs in exclusion
 of Tl from silicate minerals
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1287
_journal_page_last               1293
_journal_volume                  85
_journal_year                    2000
_chemical_formula_structural     TlAlSiO4
_chemical_formula_sum            'Al O4 Si Tl'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2n'
_symmetry_space_group_name_H-M   'P 1 1 21/n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90.01
_cell_length_a                   5.4095
_cell_length_b                   9.4232
_cell_length_c                   8.2629
_cell_formula_units_Z            4
_cell_volume                     421.200
_database_code_amcsd             0002510
_exptl_crystal_density_diffrn    5.101
_cod_original_formula_sum        'Tl Si Al O4'
_cod_database_code               9002425
_amcsd_formula_title             TlAlSiO4
The structure of agrinierite: a Sr-containing uranyl oxide hydrate mineral
Cahill, C. L.; Burns, P. C.; American Mineralogist 85 (2000) 1294–1297; doi:

data_9002426
_publ_section_title
;
 The structure of agrinierite: a Sr-containing uranyl oxide hydrate mineral
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1294
_journal_page_last               1297
_journal_volume                  85
_journal_year                    2000
_chemical_formula_sum            'Ca0.65 H14 K2 O27 Sr0.35 U6'
_chemical_name_mineral           Agrinierite
_space_group_IT_number           42
_symmetry_space_group_name_Hall  'F -2 2'
_symmetry_space_group_name_H-M   'F 2 m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   14.094
_cell_length_b                   14.127
_cell_length_c                   24.106
_cell_volume                     4799.648
_database_code_amcsd             0002511
_exptl_crystal_density_diffrn    5.561
_cod_original_formula_sum        'U6 (Sr.35 Ca.65) K2 O27 H14'
_cod_database_code               9002426
The crystal structure of namibite, Cu(BiO)2VO4(OH), and a revision of its symmetry
Kolitsch, U.; Giester, G.; American Mineralogist 85 (2000) 1298–1301; doi:

data_9002427
_publ_section_title
;
 The crystal structure of namibite, Cu(BiO)2VO4(OH), and a revision
 of its symmetry
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1298
_journal_page_last               1301
_journal_volume                  85
_journal_year                    2000
_chemical_formula_sum            'Bi2 Cu H O7 V'
_chemical_name_mineral           Namibite
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                90.10
_cell_angle_beta                 108.73
_cell_angle_gamma                107.47
_cell_formula_units_Z            2
_cell_length_a                   6.210
_cell_length_b                   7.398
_cell_length_c                   7.471
_cell_volume                     308.224
_database_code_amcsd             0002512
_exptl_crystal_density_diffrn    6.955
_cod_original_formula_sum        'Bi2 Cu V O7 H'
_cod_database_code               9002427